Bleaching of palm oil by activated local bentonite and kaolin clay from afashio, edo nigeria
Chemical and Process Engineering Research www.iiste.orgISSN 2224-7467 (Paper) ISSN 2225-0913 (Online)Vol.10, 20131Bleaching of Palm Oil by Activated Local Bentonite and KaolinClay from Afashio, Edo-NigeriaM. A. Usman*, O. Oribayo, A. A. AdebayoDepartment of Chemical Engineering, University of Lagos, Lagos 101017, NigeriaEmail: email@example.comAbstractThe bleaching potential of Afashio kaolin (AFK), from Edo state in Nigeria, for removal of pigments from palmoil was investigated in comparison with that of local bentonite (BN). Both AFK and BN were activated by acidtreatment. Batch experiments were conducted to study the effects of adsorbent dosage (2 – 8 %), contact time (0– 1.5 hr) and temperature (60 – 90oC) on pigment adsorption. Four adsorption isotherms were used to model theequilibrium data for both adsorbents (AFK and BN), namely Langmuir, Freundlich, Sips and Redlich-Petersonmodels. The Sips model provides the best correlation and adsorption occurred in monolayer. Kinetic adsorptiondata were analyzed using the pseudo-first order, pseudo-second order, and intraparticle diffusion models. Theregression results showed that the adsorption kinetics was more accurately represented by the pseudo-first orderkinetic model. Intraparticle diffusion studies reveals that pore diffusion is the controlling mechanism.Thermodynamic parameters, ∆G, ∆H and ∆S, were calculated as a function of both temperature and adsorbentdosage. The values of enthalpy change were positive and greater than 40 kJ/mol in all cases, indicating that thebleaching process is endothermic and chemisorption in nature. The results suggest that AFK could be employedas low-cost alternative for removal of pigments from vegetable oil though BN is better.Keywords: Afashio kaolin, bentonite, bleaching, equilibrium isotherms, kinetic models1. IntroductionPalm oil in its raw form contains impurities such as organic pigments, oxidation metals, trace metals and tracesoaps. For palm oil to be edible these impurities which negatively influence the taste and smell of the oil as wellas its appearance and shelf life stability, thus reducing consumer acceptance and marketability have to beremoved. Thus the refining of palm oil through adsorptive bleaching remains inevitable in the oil refiningindustry (Bockisch, 1997).Bleaching remove pigments and other unwanted compounds which negatively influence the taste of the oil bybringing into contact with a surface-active substance that adsorbs the undesired particles. Bleaching of palm oilis done by the use of adsorbents; usually activated carbons and activated bleaching earths. These bleachingearths are mainly Aluminium silicates which are usually montmorillonitic clays that exhibit adsorptive propertiesin their natural and activated state (Oboh et al., 1987).Natural clays are acquiring prominence as low-cost adsorbents over the last few decades due to their local andabundant availability and the capability to undergo modification to enhance the surface area, adsorption capacity,and range of applicability (Monvisade and Siriphannon, 2009). Therefore, in order to ameliorate the adsorptionproperties and range of applicability, a number of physical and chemical methods have been investigated tomodify the clays which including heat treatment, acid activation, treating the cationic surfactants and polymermodification (Chaisena and Rangsriwatananoon, 2004; Al-Asheh et al., 2003; Motlagh et al., 2008; James et al.,2008).Nigeria clays have been found competent in the adsorption bleaching of vegetable oil. In recent years researcheshave been carried out on clay activation and bleaching of palm oil using activated and non-activated Nigeria clay.Salawudeen et al. (2007) evaluated the effectiveness of clays from Oyo and Osun state with the view ofcomparing the adsorptive power to that found in other parts of Nigeria. Moreover, the study of activatedbleaching power of some selected Nigerian clays found in Shagamu and Ewekoro both in Ogun state; Calabar inCross River state and Nsukka, Enugu state were investigated by Oboh (1987) and reasonable percentagereduction around 80% was achieved. The bleaching performance of raw and acid activated Yola montmorilloniteclay was studied by James et al. (2008). The best bleaching performance was obtained with clay sampleactivated with 5M H2SO4 at acid to clay ratio 0.7, bleaching temperature of 120 oC and at 10 minute stirring time.At these conditions the improved clay compares favourably well in terms of bleaching performance with theimported Fuller’s earth.Many other studies have reported successful bleaching of oil using acid activated clays from across the world(Christidis et al., 1997; Komadel et al., 1990; Rozic et al., 2010; Kirali and Lacin, 2006; Srasra et al., 1989;
Chemical and Process Engineering Research www.iiste.orgISSN 2224-7467 (Paper) ISSN 2225-0913 (Online)Vol.10, 20132Novakovic et al., 2008; Foletto et al., 2011; Azeez et al., 2011; Usman et al., 2012; Ajemba and Onukwuli,2012).To the best of our knowledge, the Afashio kaolin clay (AFK) in Edo State of Nigeria has remained unexploredfor its bleaching potentials. In this study, therefore, AFK was activated by acid treatment and evaluated for thebleaching of palm oil in comparison with local bentonite (BN). The effect of such process parameters as contacttime, adsorbent dosage and temperature on bleaching of palm oil using both AFK and BN were investigated.2.0 Materials and methods2.1 MaterialsThe local kaolin clay sample was obtained from Afashio, Etsako-West Local Government, Edo State, Nigeriawhile the local bentonite clay sample was got from FIIRO (Federal Institute of Industrial Research, Oshodi) inLagos State, Nigeria. The crude palm oil was obtained locally from the Bariga, Lagos. Other materials used werehydrochloric acid, acetone (all analytical grades reagents) and distilled water.2.2 Acid ActivationThe clay samples obtained were sun-dried to make them amenable to grinding. They were then grinded with alocal mortar and pestle, and sieved using a 150 µm mesh. 50 g of the clay samples were measured, and mixedwith 250 mL of hydrochloric acid at a chosen concentration of 5 M to form slurry, and the slurry was heated at105 ◦C for 30 minutes. After slow cooling in air at room temperature, the slurry was filtered and washed free ofacid using distilled water as indicated by a pH meter. The clay was then dried at a temperature of 110◦C for 3hours, ground using mortar and pestle, sieved to 150 µm, and stored.2.3 Equilibrium adsorption studiesThe bleaching vessels were four 250 ml conical flask which were immersed in a thermostatic shaker bath. Thepalm oil (20 cm3) was heated to the desired temperature before adding the bleaching clay. The mixture continuedto be heated and stirred for 1.5 hours at the desired temperature. The hot oil and clay mixture was filtered at theend of the experiment before measuring the absorbance. The concentration of the clay in the conical flasks was2%, 4%, 6% and 8% by weight. The experiments were carried out at temperatures of 60, 70, 80 and 90 oC.2.4 Adsorption Kinetics ExperimentFor the adsorption kinetics experiment, 20cm3of crude palm oil was placed in four 250ml conical flask held in athermostatic shaker bath to reach the desired temperature before adding 0.8g of the clay samples (using anadsorbent oil ratio of 4%) which was monitored for 1.5 hours. The samples as contained in the four conicalflasks were taken out from the bath at a respective time of 15, 30, 60 and 90 min, and filtered to measure theabsorbance. The experiments were carried out at temperatures of 60, 70, 80 and 90 oC.2.5 Evaluation of the Bleaching PerformanceAt the end of each bleaching process, the content of the flask were filtered through a Whatman No.1 filter paperand the concentration in pigment of the filtrate was determined. The evaluation of the amount of pigment wasmade by UV visible spectroscopy. The samples were diluted in acetone to a concentration of 10% (v/v), and theabsorbances of the samples were determined at a wavelength of 450 nm using the UV spectrophotometer.To measure the absorbance of the unbleached palm oil, , 1 cm3of the unbleached palm oil was diluted inacetone to a concentration of 10% (v/v), and its absorbance was determined at a wavelength of 450nm using theUV spectrophotometer.The bleaching performance of the adsorbent was determined from the following equation (1):(1)Where and are the absorbance of the crude and bleached palm oil respectively3.0 Results and discussion3.1 Adsorption Kinetics3.1.1 Effect of Contact TimeThe kinetic studies were carried out at 60, 70, 80, and 90 oC with an adsorbent oil ratio of 4%. The adsorbentsused for kinetic studies were AFK and BN activated with 5M hydrochloric acid solution as reported in Figure 1and Figure 2. It is observed that the bleaching efficiencies of the adsorbents vary with the temperature for all thebleaching efficiency curves i.e. the bleaching efficiency increases with the increase in temperature for all theadsorbent used herein. For the bleaching of the palm oil, both activated clays present similar evolution of thebleaching capacities versus time. The bleaching of oil is fast in the first 30 mins and progresses much moreslowly thereafter. And towards approaching a contact time of 90 min (1.5h), the bleaching efficiency begins tostabilize or become steady as the medium approaches equilibrium.
Chemical and Process Engineering Research www.iiste.orgISSN 2224-7467 (Paper) ISSN 2225-0913 (Online)Vol.10, 20133Figure 1: Kinetics of bleaching palm oil at different temperatures by BNFrom Figure 1, unlike the bleaching efficiency curve of 60 oC which attained an optimum value after 60 mins, itcan be deduced that a bleaching efficiency greater than 81.4% can still be obtained for the bleaching efficiencycurve of 90 oC after a total contact time of 90 mins i.e. with an increase in the contact time, the optimumbleaching efficiency can be attained while that of local kaolin clay, likewise, as seen in Figure 2, gives ableaching efficiency of 62.4% at a temperature of 90 oC and contact time of 90 min.Figure 2: Kinetics of bleaching palm oil at different temperatures by AFK3.1.2 Effect of variation in adsorbent dosageFigure 3 and 4 represents the plot of bleaching efficiency versus adsorbent dosage. The clay dosage was variedfrom an adsorbent oil ratio of 2% to 8%.It was observed that increasing the clay dosage increased the bleachingefficiency for both AFK and BN; however, the results clearly indicate that the bleaching efficiency increases toan optimum value from which further increase in the adsorbent dosage has no significant effect on them. Theattainment of a steady bleaching efficiency beyond the optimum as particular to both local clays can beexplained by the fact that adsorption equilibrium has been reached between the adsorbent/oil mixtures, thereby,preventing further pigment removal by the excess adsorbent dosage.Figure 3: Variation of the bleaching efficiency of the adsorbent as a function of the adsorbent used for palm oilbleaching for BN
Chemical and Process Engineering Research www.iiste.orgISSN 2224-7467 (Paper) ISSN 2225-0913 (Online)Vol.10, 20134Figure 4: Variation of the bleaching efficiency of the adsorbent as a function of the adsorbent used for thebleaching of palm oil for AFK3.2 Adsorption IsothermAdsorption isotherm describes the equilibrium of the sorption of the palm oil impurities at constant temperature.To evaluate the nature of adsorption, the experimental isotherm data were fitted by model isotherm equationsnamely; the Langmuir (1906) equations (2, 3), Freundlich (1918) equations (4, 5), Sips (Sips, 1948) equations (6,7) and Redlich–Peterson (Redlich and Peterson, 1959) equations (8, 9) in terms of absorbance (X) andconcentration (C) respectively (Foo and Hameed, 2010; Kumar and Porkodi, 2006; Toor and Jin, 2012).
Chemical and Process Engineering Research www.iiste.orgISSN 2224-7467 (Paper) ISSN 2225-0913 (Online)Vol.10, 20135Where X/m = qe, and Xe = CeX is amount of adsorbed solute, Xe is amount of unadsorbed solute, m is grams of adsorbent, a and b areLangmuir isotherm constant and Freundlich isotherm constant are n and K. Figures 5, 6, 7 and 8 shows theFreundlich, Langmuir, Sips, Redlich-Peterson isotherm respectively for the bleaching of palm oil with theactivated clays. The isotherm model parameters and the statistical fits of the adsorption data to these models ascalculated are presented in Table 1. It was observed that Sips model adequately described the adsorption datawith best linear fit and greater regression coefficient values for the AFK and BN.Figure 5: Freundlich isotherm for the bleaching of palm oil with [A] AFK and [B] BN at various temperaturesFigure 6: Langmuir isotherm for the bleaching of palm oil with [A] AFK and [B] BN at various temperatures
Chemical and Process Engineering Research www.iiste.orgISSN 2224-7467 (Paper) ISSN 2225-0913 (Online)Vol.10, 20136Figure 7: Sips isotherm for the bleaching of palm oil with [A] AFK and [B] BN at various temperaturesFigure 8: Redlich - Peterson isotherm for the bleaching of palm oil with [A] AFK and [B] BN at varioustemperaturesTable 1: Langmuir, Freundlich and Sips isotherm constants for the bleaching of palm oil with AFK and BNAFK BNIsothermModelsParameterTemperature(oC) Temperature(oC)60oC 70oC 80oC 90oC 60oC 70oC 80oC 90oCFreundlichK 0.6079 0.2396 0.379 2.063 2.3878 18.638 27.759 9.57191/n 0.1143 0.2567 0.4671 0.2988 0.2289 0.1832 0.2436 0.3590R20.9399 0.8714 0.9749 0.9999 0.9924 0.9953 0.9912 0.8684Langmuira -0.007 -0.023 -0.094 -0.058 -0.036 -0.032 -0.055 -0.099b -1.153 -1.021 -0.947 -1.538 -1.501 -1.961 -2.555 -2.615R20.9491 0.8057 0.8788 0.9751 0.9554 0.9887 0.9967 0.7766Sipsa*10-3-9.8 -2.66 -7.9 -6.23 -4.2 -3.98 -6.43 -9.97b -1.023 -1.008 -1.014 -1.076 -1.067 -1.109 -1.156 -1.167R20.9558 0.8718 0.9329 0.9745 0.9620 0.9854 0.9937 0.9098Redlich- a -0.005 -.0169 -0.075 -0.050 -0.030 -0.028 -0.055 -0.11Peterson b -1.095 -1.003 -0.928 -1.312 -1.294 -1.543 -1.825 -1.819R20.9488 0.8035 0.8825 0.9798 0.9598 0.9909 0.9983 0.76143.3 Adsorption ThermodynamicsThermodynamic behavior of the adsorption process was evaluated by the following thermodynamic parametersincluding the change in free energy (∆G), enthalpy (∆H), and entropy (∆S).These parameters were obtainedusing the following equations:
Chemical and Process Engineering Research www.iiste.orgISSN 2224-7467 (Paper) ISSN 2225-0913 (Online)Vol.10, 20137(10)where R is the universal gas constant (8.314 (J/mole) K), T is temperature(K), and Kd is the distributioncoefficient for the adsorption.Table 2: Thermodynamic behavior parameter of the adsorption process for the bleaching of palm oil with AFKand BNAFK BNParameterAdsorbent Dosage Adsorbent Dosage2% 4% 6% 8% 2% 4% 6% 8%∆H 45.3271 51.54846 50.28307 52.01155 41.50515 39.50647 39.53253 43.3201∆S 0.1230 0.1434 0.1420 0.1477 0.1224 0.1185 0.1160 0.1316R2 0.9129 0.943 0.9689 0.9675 0.9814 0.9882 0.9731 0.9882AFK BNThermo-dynamic ParameterTemperature(oC) Temperature(oC)60oC 70oC 80oC 90oC 60oC 70oC 80oC 90oC∆G2% 848.2 -468.7 -1986 -2702.3 3907.8 3761.1 2118.3 289.94% 33.2 -1002.6 -2542.8 -3396.6 3424.1 3042.4 779.3 -642.26% -277.1 -1299.6 -2948.9 -3578.9 2824.32 1980.93 -211.4 -11868% -622.8 -1579.1 -3271.4 -4455.2 2642.33 1803 -482.4 -1528In this study, the positive ∆His an indicator of endothermic nature of the adsorption and also its magnitude givesinformation on the type of adsorption, which can be either physical or chemical. The enthalpy of adsorption,ranging from 40 to 400 kJ/mole corresponds to chemisorption (activated adsorption). Chemisorption occurs
Chemical and Process Engineering Research www.iiste.orgISSN 2224-7467 (Paper) ISSN 2225-0913 (Online)Vol.10, 20138when the intermolecular attractive forces between molecules of the adsorbate itself are greater than thosebetween molecules of adsorbate and adsorbent. In this study, the adsorption heat of the pigments is in range ofchemisorption. Therefore, the ∆H values show that the adsorption of pigments on the local clays takes place viachemisorption. The positive range of ∆S value suggests an increase in the randomness at adsorbate-solutioninterface during the adsorption process. Also the decrease in ∆G values with increasing temperature shows adecrease in feasibility of adsorption at higher temperatures.3.4 Adsorption kinetics modelsThe effect of contact time on the bleaching efficiency of AFK and BN activated with 5M hydrochloric acid asreflected in Figure 1 and 2, were tested with three kinetic models in order to examine the controlling mechanismof the adsorption process which are Pseudo-first order kinetic (Lagergren, 1898), pseudo-second order kinetic(Ho and McKay, 1999) and intraparticle diffusion model (Webber Jr and Morriss, 1963).The respective differential and linear forms of the equations are as given below:Intraparticle diffusion model (17)Figure 8: Pseudo-first order kinetics for the adsorption of palm oil pigments onto [A] AFK and [B] BN
Chemical and Process Engineering Research www.iiste.orgISSN 2224-7467 (Paper) ISSN 2225-0913 (Online)Vol.10, 20139Figure 9: Pseudo-second order kinetics for the adsorption of palm oil pigments onto [A] AFK and [B] BNFigure 9: Intraparticle diffusion for the adsorption of palm oil pigments onto [A] AFK and [B] BN
Chemical and Process Engineering Research www.iiste.orgISSN 2224-7467 (Paper) ISSN 2225-0913 (Online)Vol.10, 201310Table 3: The kinetic parameters evaluated for palm oil pigment adsorption onto local claysAFK BNIsothermModels ParameterTemperature(oC) Temperature(oC)60oC 70oC 80oC 90oC 60oC 70oC 80oC 90oCPseudo-First-Orderqe (exp)0.32 0.495 0.6425 0.8488 0.7163 0.7788 0.9175 1.0013qe (calc)0.3064 0.4937 0.9112 0.997 0.8111 0.8089 0.9322 0.9521k10.0191 0.0164 0.0216 0.053 0.0339 0.0297 0.0265 0.0246R2 0.9851 0.9873 0.9653 0.8787 0.9636 0.9592 0.9946 0.9563Pseudo-Second-Orderqe (exp)0.32 0.495 0.6425 0.8488 0.7163 0.7788 0.9175 1.0013qe (calc)0.6961 0.6877 0.7531 0.8564 0.6961 0.6877 0.7531 0.8564k20.0822 0.1209 0.1045 0.1304 0.0822 0.1209 0.1045 0.1304R2 0.7122 0.8009 0.771 0.9058 0.7122 0.8003 0.771 0.9058IntraparticleDiffusionqe (exp)0.32 0.495 0.6425 0.8488 0.7163 0.7788 0.9175 1.0013C -0.0142 -0.0708 -0.0432 -0.0846 -0.0383 -0.0387 -0.0189 -0.0026K30.0324 0.0751 0.0498 0.0896 0.0788 0.0959 0.0828 0.105R2 0.9712 0.9063 0.9248 0.9333 0.9755 0.9689 0.9812 0.9998The associated kinetic parameters have been evaluated from the slopes and intercepts of the respective linearplots of the pseudo-first order, pseudo-second order kinetic equation and intraparticle diffusion with the valuesas shown in Table 3. Comparison of the analyzed data based on the linear regression coefficient (R2) values,showed that the experimental data is best described by the pseudo-first order kinetic model for both adsorbents.Intraparticle diffusion study show straight line passing through the origin with high correlation coefficient forboth adsorbents. Therefore the intraparticle diffusion is the dominating mechanism for the adsorption process.4.0 ConclusionThe kinetic and equilibrium studies of the adsorptive purification of palm oil using hydrochloric acid activatedAFK and BN has been successfully investigated. The adsorption of pigments onto the clay surfaces increasedwith temperature, adsorbent dosage and contact time.Langmuir, Freundlich,Sips and Redlich–Peterson adsorption models were applied to describe the experimentalequilibrium isotherms. The Sips model agreed well with the equilibrium adsoption data with R2range of 0.9063to 0.9998, while the Langmuir, Freundlich, and Redlich–Peterson equation gave a slightly poorer fit.The heatevolved during adsorption was recorded as 39.52 to 43.32 kJmol-1and 45.33 to 51.55 kJmol-1for the localactivated bentonite and kaolin clay respectively. These values are greater than 40 kJmol-1which is an indicationof activated adsorption (chemisorption) between the adsorbate and adsorbent. The kinetic study performed basedon pseudo-first-order, pseudo-second-order and intraparticle diffusion indicates that the pseudo-first orderkinetic model better represents the bleaching process while intraparticle diffusion is the dominating mechanismfor the adsorption process.The thermodynamic parameters, namely ∆H, ∆S and ∆G showed that adsorption of pigments onto the localactivated bentonite and kaolin clay respectively under the examined conditions was spontaneous andendothermic.The optimum bleaching condition was equivalent to a bleaching efficiency of 81.4% and 62.4% for the localactivated bentonite and kaolin clay respectively, consequently indicating that the clays have potential asbleaching earth/adsorbent under this condition. We infer that Afashio clay from Edo state in Nigeria can beconverted into potential adsorbents for bleaching of palm oil, which can represent economy added value.
Chemical and Process Engineering Research www.iiste.orgISSN 2224-7467 (Paper) ISSN 2225-0913 (Online)Vol.10, 201311ReferencesAjemba R.O. and Onukwuli O.D. (2012). Response surface optimization of palm oil bleaching usinghydrochloric acid activated Ukpor clay. European Journal of Scientific Research, 82(3), 325 – 339.Al-Asheh, S., Banat, F., Abu-Aitah, L. (2003). Adsorption of phenol using different types of activated bentonites,Separation and Purification Technology, 33(1), 1-10.Aziz, B.K., Abdullah, M.A., Jubrael, K.J. (2011). Acid activation and bleaching capacity of some local clays fordecolourizing used oils. Asian Journal of Chemistry, 23(6), 2449 – 2455.Bockisch, M., Fats and Oils Handbook, AOCS Press, pp. 613-615, 1997Chaisena, A. and Rangsriwatananoon, K. (2004). Effects of thermal and acid treatments on some physico-chemical properties of Lampang diatomite. Suranaree Journal of Science Technology,11, 289–299.Christidis, G.E., Scott, P.W., Dunham, A.C. (1997). Acid activation and bleaching of bentonites from the islandsof Milos and Chios, Aegean, Greece. Applied Clay Science, 12, 329 – 347.Foletto, E. L., Colazzo, G. C., Volzone, C., Porto, L. M. (2011). Sunflower oil bleaching by adsorption ontoacid-activated bentonite. Brazilian Journal of Chemical Engineering, 28(1), 169 – 174.Foo, K.Y., Hameed, B.H.(2010). Review-insights into the modelling of adsorption isotherm systems. ChemicalEngineering Journal, 156, 2 – 10.Freundlich, H.M.F. (1906). Uber die adsorption in losungen. Z. Phys. Chem., 57, 385 – 470.Ho, Y.S., McKay, G. (1999). Pseudo-second order model for sorption processes. Process Biochem., 34, 451 -465.James, O. O., Mesubi, M. A., Adekola, F. A., Odebunmi, E. O., Adekeye, J. I. D., Bale, R. B. (2008). Bleachingperformance of a Nigerian (Yola) bentonite. Latin American Applied Research, 38, 45 – 49.Kirali, E. G., Lacin O. (2006). Statistical modelling of acid activation on cotton oil bleaching by Turkishbentonite. Journal of Food Engineering, 75, 137 – 141.Komadel, P., Schmidt, D., Madejova, J., Cicel, B. (1990). Alteration of smectites by treatments withhydrochloric acid and sodium carbonate solutions. Applied Clay Science, 5, 113 – 122.Kumar, K.V., Porkodi, K. (2006). Relation between some two- and three-parameter isotherm models for thesorption of methylene blue onto lemon peel. Journal of Hazardous Material, 138, 633 – 635.Lagergren, S. (1898). About the theory of so-called adsorption of soluble substances. Kungliga SvenskaVetenskapsakademiens, Handlinger, 24, 1-39.Langmuir, I. (1918). The adsorption of gases on plane surfaces of glass, mica and platinum. Journal of AmericanChemical Society, 40, 1361 – 1403.Monvisade, P, Siriphannon, P. (2009). Chitosan intercalated montmorillonite: preparation, characterization andcationic dye adsorption. Applied Clay Science, 42( 3-4), 427-431.Motlagh, M, Rigi, A, Yuzbashi, A. (2008). To evaluate an acid activated bentonite from Khorasan (Iran) for useas bleaching clay. International Journal of Engineering Science, 19(5-2), 83-87, 2008.Novakovic, T., Rozic, L., Petrovic, S., Rosic, A. (2008). Synthesis and characterization of acid-activated Serbiansmectite clays obtained by statistically designed experiments. Chemical Engineering Journal, 137, 436 – 442.Oboh, A.O., Aworh, O.C. and Agagu, O.K. (1987). The use of Nigerian clays in vegetable oil refining:Evaluation of some Nigerian clays as potential bleaching earths. Nigerian Food Journal, 5, 42-51.Redlich, O., Peterson, D.L. (1959). A useful adsorption isotherm. Journal of Physical Chemistry, 63, 1024 –1029.Rozic, L., Novakovic, T., Petrovic S. (2010). Modeling and optimization process parameters of acid activation ofbentonite by response surface methodology. Applied Clay Science, 48, 154 – 158.Salawudeen, T.O, Dada, E.O, Alagbe, S.O. (2007). Performance evaluation of Acid Treated Clays for Palm oilbleaching. Journal of Engineering and Applied Sciences, 2(11), 1677-1680.Sips, R. (1948). Combined form of Langmuir and Freundlich equations. Journal of Chemical Physics, 16, 490 –495.Srasra, E., Bergaya, F., Van Damme, H., Ariguib, N.K. (1989). Surface properties of an activated bentonite –decolorisation of rape-seed oils. Applied Clay Science, 4, 411 – 421.Toor, M., Jin, B. (2012). Adsorption characteristics, isotherm, kinetics, and diffusion of modified naturalbentonite for removal of diazo dye. Chemical Engineering Journal, 187, 79 – 88.Usman M.A., Ekwueme V.I., Alaje T.O., Mohammed A.O. (2012). Characterization, acid activation andbleaching performance of Ibeshe clay, Lagos, Nigeria. ISRN Ceramics, vol. 2012, article ID 658508, 5 pages, doi:10.5402/2012/658508.Webber Jr, W.J., Morriss, J.C. (1963). Kinetics of adsorption on carbon from solution. J. Saint. Eng. Div. Am.Soc. Civ. Eng., 89, 31 – 60.